Fluorine Substitution Induced High T<sub>c</sub> of Enantiomeric Perovskite Ferroelectrics: ( R) - and ( S) -3-(Fluoropyrrolidinium)MnCl<sub>3</sub>.
Ai, Yong; Chen, Xiao-Gang; Shi, Ping-Ping; Tang, Yuan-Yuan; Li, Peng-Fei; Liao, Wei-Qiang; Xiong, Ren-Gen; Journal of the American Chemical Society 141 (2019) 4474–4479; doi:10.1021/jacs.9b00886

data_4127488
_publ_section_title
;
 Fluorine Substitution Induced High T<sub>c</sub> of Enantiomeric
 Perovskite Ferroelectrics: ( R) - and ( S)
 -3-(Fluoropyrrolidinium)MnCl<sub>3</sub>.
;
_journal_issue                   10
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              4474
_journal_page_last               4479
_journal_paper_doi               10.1021/jacs.9b00886
_journal_volume                  141
_journal_year                    2019
_chemical_absolute_configuration rm
_chemical_formula_moiety         'Cl3 Mn, C4 H9 F N'
_chemical_formula_sum            'C4 H9 Cl3 F Mn N'
_chemical_formula_weight         251.41
_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_Hall           'P 2yb'
_space_group_name_H-M_alt        'P 1 21 1'
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 112.474(8)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.6220(5)
_cell_length_b                   6.4880(3)
_cell_length_c                   9.5948(7)
_cell_measurement_reflns_used    2283
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      30.5490
_cell_measurement_theta_min      3.8980
_cell_volume                     438.44(5)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.800
_diffrn_measurement_device_type  'XtaLAB Synergy R, DW system, HyPix'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0110
_diffrn_reflns_av_unetI/netI     0.0162
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.800
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            2787
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.793
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.623
_diffrn_reflns_theta_min         2.892
_exptl_absorpt_coefficient_mu    2.361
_exptl_absorpt_correction_T_max  0.554
_exptl_absorpt_correction_T_min  0.497
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.14e (Rigaku Oxford Diffraction, 2018)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    1.904
_exptl_crystal_description       needle
_exptl_crystal_F_000             250
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.28
_exptl_crystal_size_min          0.25
_refine_diff_density_max         1.312
_refine_diff_density_min         -0.665
_refine_diff_density_rms         0.127
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.04(5)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.158
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     92
_refine_ls_number_reflns         1729
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.157
_refine_ls_R_factor_all          0.0457
_refine_ls_R_factor_gt           0.0440
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0819P)^2^+0.3843P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1317
_refine_ls_wR_factor_ref         0.1344
_reflns_Friedel_coverage         0.838
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     0.785
_reflns_number_gt                1612
_reflns_number_total             2708
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ja9b00886_si_004.cif
_cod_data_source_block           P21
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_database_code               4127488
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              81140
_shelx_hkl_checksum              85221